#------------------------------------------------------------------------------
#$Date: 2014-08-15 21:14:22 +0300 (Fri, 15 Aug 2014) $
#$Revision: 23 $
#$URL: svn+ssh://sauliusg@svn.code.sf.net/p/propcif/code/trunk/cif/1/1000066.mpod $
#------------------------------------------------------------------------------
#
# This file is available in the Material Properties Open Database (MPOD),
# http://www.materialproperties.org/
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_1000066
_cod_database_code               1010298
_structure_refined 'no'
_mpod_phase_name ?
_mpod_phase_generic_name 'Nd:SGGM'
_chemical_formula_sum 'Nd0.0136 Sr0.92 Gd1.01 Ga2.88 O7'
_mpod_symmetry_point_group_name_H-M '-4 2 m'
_cell_length_a  7.972
_cell_length_c  5.251
loop_
_publ_author_name
'Zhang, Y.Y.'
'Zhang, H.J.'
'Yu, H.H.'
'Wang, J.Y.'
'Gao, W.L.'
'Xu, M.'
'Sun, S.Q.'
'Jiang, M.H.'
'Boughton, R.I.'
_publ_section_title
;
 Synthesis, growth, and characterization of Nd-doped SrGdGa3O7 crystal
;
_journal_name_full               'Journal of Applied Physics'
_journal_volume                  108
_journal_issue                   6
_journal_article_reference       063534
_journal_pages_number            10
_journal_year                    2010
_mpod_phase_density 5634

data_1000066a
_prop_measurement_method LPM
_prop_thermal_conductivity_kappaij 'kappaij'
_prop_thermal_diffusivity_kappadij 'kappadij'
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
_prop_conditions_temperature
kappaij 11 1.59 303.1
kappaij 22 1.59 303.1
kappaij 33 ? 303.1
kappaij 11 2.12 560.6
kappaij 22 2.12 560.6
kappaij 33 ? 560.6
kappaij 11 ? 304
kappaij 22 ? 304
kappaij 33 1.40 304
kappaij 11 ? 560.2
kappaij 22 ? 560.2
kappaij 33 1.96 560.2
kappadij 11 0.00000067 303
kappadij 22 0.00000067 303
kappadij 33 0.00000059 303

data_1000066b
_prop_conditions_temperature_range_begin 303
_prop_conditions_temperature_range_end 773
_prop_measurement_method SCXD
_prop_thermal_expansion_alphaij 'alphaij'
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
alphaij 11 5.32
alphaij 22 5.32
alphaij 33 5.65

data_1000066c
_prop_conditions_temperature 303
_prop_measurement_method DSC
_prop_heat_capacity_C 'C'
loop_
_prop_data_label
_prop_data_value
C 0.419

data_1000066d
_prop_measurement_method MDT
_prop_optical_index_ordinary_no 'no'
_prop_optical_index_extraordinary_ne 'ne'
loop_
_prop_data_label
_prop_data_value
_prop_conditions_wavelength
no 2.0379258 0.2537
no 1.9012401 0.363
no 1.8793089 0.4047
no 1.8670582 0.4358
no 1.8543279 0.480
no 1.8414330 0.5461
no 1.8357980 0.5875
no 1.8296930 0.6438
no 1.8246548 0.7065
no 1.8170938 0.8521
no 1.8118757 1.014
no 1.8033156 1.530
no 1.7946656 2.325
ne 2.0616061 0.2537
ne 1.9066923 0.363
ne 1.8864119 0.4047
ne 1.8749420 0.4358
ne 1.8629145 0.480
ne 1.8506377 0.5461
ne 1.8451414 0.5875
ne 1.8393703 0.6438
ne 1.8345550 0.7065
ne 1.8272175 0.8521
ne 1.8222021 1.014
ne 1.8139621 1.530
ne 1.8057108 2.325
